Esthetic orthodontic brackets /certified fixed orthodontic courses by Indian dental academy
INDIAN DENTAL ACADEMY
Leader in continuing dental education
As the number of adults seeking orthodontic
care increased, orthodontists felt the need
to provide their patients with more esthetically
This perceived need motivated manufacturers to
provide acceptable esthetic brackets, including the
Ceramics are materials that are both very rigid
and brittle, that is, nonductile.
The Effect of the Manufacturing Process on the
Physical Characteristics of Ceramic Brackets
Although the term ceramics encompasses different
compounds, most currently available ceramic brackets
are composed of aluminum oxide.
Two basic types of brackets exist, based on two
different manufacturing processes.
The polycrystalline brackets are made of sintered or
fused aluminum oxide particles.
The process begins by blending the particles with a
This mixture is then molded into a shape from
which the critical parts of the brackets can be cut.
The molded part is then fired at a temperature that
allows the binder to be burnt out and the aluminum
oxide particles to fuse but not melt.
This firing process is called sintering.
This molding/sintering process is relatively
inexpensive, making it a popular manufacturing
Unfortunately, the process results in both structural
imperfections at grain boundaries and the
incorporation of trace amounts of impurities.
These slight imperfections and impurities, even in
quantities as low as 0.001%, can serve as foci for
crack propagation under stress.
This could lead to fracturing of the bracket.
Monocrystalline ceramic brackets also are
manufactured from aluminum oxide.
In this process, the oxide particles are melted and
then cooled slowly, permitting complete
This process minimizes the stress-inducing impurities
and imperfections found in the polycrystalline
The orthodontic bracket is then milled into shape from
the single crystal of aluminum oxide.
This is a more difficult and expensive manufacturing
process, because of the hardness of the ceramic
Milling and the presence of sharp corners introduce
their own stresses on the material and also
predispose the bracket to fracture.
Optical Properties of Ceramic Brackets
The optical properties of ceramics provide the only
advantage over stainless steel brackets.
The larger the ceramic grains, the greater the clarity
However, when the grain size reaches about 30 |im,
the ceramic material becomes weaker.
The grain boundaries and impurities that are present
in polycrystalline ceramics reflect light, resulting in
some degree of opacity.
The monocrystalline brackets, however, are
The clear appearance is the result of two factors:
1.Reduction of grain boundaries and
2.Having fewer impurities introduced during the
Whether the difference between the optical properties
of the opaque and clear ceramics is significant from
an esthetic point of view is based on the personal
preference of the clinician.
This is particularly true because ceramic brackets in
the oral environment can be affected by color
pigments for example, in tea, coffee, and wine.
The Effects of Hardness of Ceramics on Various
Aspects of Orthodontic Treatment
Four important side effects that ceramic brackets
have on orthodontic treatment have been identified:
1. Ceramic is the third hardest material known to
humans. Therefore, brackets in contact with opposing
teeth can cause wear of the relatively softer enamel.
2. Because aluminum oxide is much harder than
stainless steel, the slot in the ceramic bracket shows
minimum wear during sliding mechanics. However,
nicks occur in the relatively softer metal arch wires,
which increases friction.
3. When using sliding mechanics, the relatively rough
surfaces of the ceramic slot significantly increases
frictional resistance when compared with stainless
A decrease in the efficiency of canine retraction was
estimated at 25% to 30% when ceramic and stainless
steel brackets were compared.
4. The "fracture toughness" (the ability of a material to
resist fracture) of ceramic brackets is much lower than
For example, the elongation (deformation) of stainless
steel is approximately 20% before it finally fails, and
the elongation of sapphire before failure does not
exceed 1%. Compared with a metal bracket, the
ceramic bracket is more susceptible to fracture when
orthodontic forces are applied to it.
As a result, stresses introduced during Ligation and
arch wire activation, forces of mastication and
occlusion, and forces applied during bracket removal
are all capable of creating cracks in the ceramic
brackets which maywww.indiandentalacademy.com
Types of Retention Mechanisms Incorporated in the Ceramic
Aluminum oxide, from which ceramic brackets are made, is an
As a result, it cannot chemically adhere directly to any of the
currently available bonding resins.
For these reasons, two different basic mechanisms were
developed by which ceramic brackets could be attached to the
The first method is by mechanical retention achieved by
indentations or recesses in the bracket base, much like the mesh
on the base of metal brackets. These indentations provide a
mechanical interlocking with the resin adhesive.
The second method is by employing an intermediate
layer of glass on the bracket base and using a silane
coupler to obtain a chemical bond between the
bracket and the adhesive.
There are therefore three different retention
mechanisms by which ceramic brackets can be
attached to the bonding agent –
1. Chemical retention using silane,
2. Mechanical retention, and
3. A combination of both methods.
The Effects of the Retention Mechanism on Bond
The possibility of enamel damage when debonding
ceramic brackets may be attributable to many factors.
A significant factor is the increased bond strength at the
A number of studies have shown that chemically
retained ceramic brackets produce a significantly
stronger bond strength, compared with conventional
Increased bond strength with ceramic brackets resulted
in bond failure at the enamel-adhesive interface, rather
than at the "safer" bracket-adhesive interface, which is
fairly common with metal brackets.
Failure at the enamel-adhesive interface results in an
increased incidence of enamel fractures.
The latter is of concern to patients and clinicians, as
well as to manufacturers.
As a result, some manufacturers have added grooves,
recesses, or a rough surface onto the base of their
ceramic brackets to increase the surface area and
allow for more mechanical interlocking and less need
for chemical adhesion between the bracket and the
Guess et al suggested that the mechanical interlocking
in the bracket base provided adequate strength and
that the additional chemical bond provided by the
silane was unnecessary.
As debonding complications occurred, partly because
of the high bond strengths, some manufacturers
developed ceramic brackets designed to reduce the
bond strengths of the brackets.
Their brackets have mechanical retention only, or the
silane coupler was applied only in the mechanical
Some investigators contend that the use of a silane
coupler, in combination with the mechanical retention,
increased the bracket's bond strength.
Others considered that this combination of chemical
and mechanical retention does not alter the tensile
strength but significantly decreased the shear
strength when compared with that of the chemically
backed ceramic brackets.
The Effect of Enamel Surface Conditioning on
A number of factors related to surface conditioning
may influence bond strength. These include acid
etching and crystal growth.
Adhesion of the resin to the etched enamel surface
occurs through mechanical retention.
Etching the enamel surface with acid leaves a
microscopic honeycomb lattice appearance.
This is the result of preferential dissolution between
the prism periphery and its core, producing
microspaces or porosities in the enamel surface.
Along with increasing the total enamel surface area
available for mechanical bonding, acid etching
increases the wettability of the surface.
This facilitates the flow of the resin material over the
enamel surface, allowing greater penetration of
resin tags into the undercuts of the etched surface.
After polymerization, the adhesive resin tags form a
tightly interlocking mechanical bond with the etched
It has been suggested that reducing either acid
etching concentrations or etching time may decrease
Research has shown that varying acid etching
concentrations from 5% to 37% did not significantly
affect bond strength.
Furthermore, reducing etching times from 60 to 15
seconds, and even to 10 seconds, did not
significantly change either the bond strength or the
bond failure of ceramic brackets.
However, reducing the etching time to 5 seconds
resulted in an inadequate bond.
These results indicate that reducing etching time will
not significantly aid the clinician at the time of the
debonding of ceramic brackets (unless times are
reduced to less than 5 seconds).
Smith proposed an alternative method for preparing
the enamel surface for the direct bonding of
orthodontic attachments, which he called crystal
It has been shown that polyacrylic acid, containing
residual sulfate ions, reacted with the enamel surface
to produce a deposit of white spherulitic crystalline
calcium sulfate to which the adhesive resin bonds.
The crystals were identified as calcium sulfate
dihydrate, CaSO4 • H2O (gypsum).
The crystal growth bonding technique has several
advantages over the phosphoric acid etch technique;
(1) the enamel surface is not significantly damaged,
(2) debonding and enamel cleanup are easier,
(3) there is minimal loss of the outer fluoride rich
enamel layer, and
(4) few if any resin tags are left in the enamel after
Maijer and Smith compared the conditioning of
enamel by the acid-etch technique with the crystal
They concluded that conditioning with polyacrylic acid
had a bond strength comparable to that of acid-etching
with phosphoric acid, both in the laboratory and
However, other researchers found that bond strengths
with the use of crystal growth conditioning was much
weaker than that of the conventional acid etching
It should be noted that the polyacrylic acids used in the
latter experiments were not of the same formula as that
used by Maijer and Smith.
One problem with the crystal growth technique is that
it is operator sensitive.
Inadequate washing will not completely remove the
polyacrylic acid solution and this will result in a weaker
It has also been suggested that rinsing too vigorously
may remove the crystals and therefore reduce bond
Burkey found that the bond strengths obtained with
the use of polyacrylic acid are nearly equal to those
obtained by conventional acid etching techniques,
even when the crystalline structure was not
Although it is recommended that a 30-second rinse be
used, others found that it took approximately 1 minute
to ensure the complete removal of the polyacrylic acid
and still preserve the crystals.
The addition of red coloring to the polyacrylic acid
product made it possible to assure the removal of all
the excess polyacrylic acid.
In general, the use of polyacrylic enamel conditioner
in the crystal growth technique resulted in a reduced
debonding strength when compared with the use of
phosphoric acid in the conventional acid etch
However, the "reduced" strength was still above the
minimum bond strength of 60 kg/cm2 recommended
by Reynolds as being adequate for clinical usage.
This relative reduction in bond strength might be
advantageous when debonding ceramic brackets,
because it reduces the stress on the enamel surface.
With the use of the crystal growth enamel conditioning
method, bond failure still occurs at the enameladhesive interface.
In general, this is considered the least desirable
location for bond failure because of the increased risk
for enamel damage.
However, with the use of polyacrylic acid conditioner,
the bond actually fails within the crystals and not at
the enamel surface, minimizing the probability of
There are essentially two groups of adhesives used for
bonding orthodontic brackets to enamel, acrylic and
Acrylic resins consist of a methylmethacrylate
monomer and an ultra fine polymer powder.
Similar to self-curing acrylic, activation is usually
achieved by a catalyst.
Some investigators believe that acrylic resins are
relatively poor orthodontic bracket adhesives because
they do not possess adequate bond strength.
Diacrylic resins are based on an acrylic modified epoxy
resin, generally referred to as bis-GMA (bisphenol A
The major difference between diacrylic and acrylic
resins is that the latter can form only linear polymers.
However, the diacrylic resins may be polymerized also
by cross-linking into a three dimensional network.
This cross-linking contributes to the greater strength,
low water absorption, and less polymerization
shrinkage of the diacrylic resins.
The Effects of the Adhesive Additives on Bond
Diacrylic resin adhesives are available in either filled or
Often an orthodontic bonding system will contain both
The best example of the unfilled resin is the sealant
that is placed on the etched enamel surface.
In most cases for bracket bonding this step is followed
by applying a filled resin that provides for increased
The filler is usually an inorganic material and is used
mainly to minimize the deformation and strengthen the
matrix of the adhesive.
The dimensionally stable filler is combined with the
dimensionally unstable resin to reduce the coefficient
of thermal expansion of the resin matrix for it to
approximate that of enamel.
The filler can vary in composition, size of particle, and
These factors, plus any added chemical modifiers, can
significantly influence abrasion resistance, viscosity,
and hardness of thewww.indiandentalacademy.com
The fillers currently used in orthodontic adhesives
are composed of either quartz or silica glass.
The quartz is a harder material, lending itself to less
wear of the composite.
This is an important factor in operative dentistry but
less so in orthodontics.
The softer silica glass may be advantageous in
orthodontics at the time of debonding, because it
may cause less wear of the debonding plier and also
make it easier for the clinician to clean the residual
adhesive from the www.indiandentalacademy.com
The particle size of the filler can significantly influence
the properties of the adhesive.
Orthodontic adhesives may contain one of two types
of fillers, large particles of highly variable diameter
ranging from 3 to 20u, ie, macrofilled, or submicron
filler particles with an average diameter ranging
between 0.2 and 0.3 urn, ie, microfilled.
The macrofilled resins impart abrasion resistance
properties, and the microfilled resins are more prone
to abrasion, therefore yielding a smoother surface.
Zachrisson and Brobakken showed clinically that
bonding brackets with a microfilled adhesive was
more hygienic because of less plaque retention on
the smoother adhesive surface.
Adhesives also can vary in the percentage of filler
The earlier orthodontic adhesives were heavily filled
composites (60% to 75% filled).
This caused an increase in the strength of the
More recently, lightly filled adhesives (20% to 30%
filled) were developed to overcome some of the
difficulties encountered during the removal of ceramic
It has been repeatedly demonstrated when debonding
metal brackets that highly filled diacrylic resins, when
compared with lightly filled resins, provided higher
Although many practitioners use heavily filled
adhesives because of their added strength, the recent
trend has been toward the use of lightly filled
In general, when using polyacrylic acid enamel
conditioner, the type of adhesive used, whether filled
or unfilled, was of secondary importance in influencing
When using a phosphoric acid etch, highly filled
adhesive provided a debonding strength twice that of
the lightly filled adhesive.
However, the findings have also indicated that some
unfilled adhesives may have a debonding strength
comparable to those of the highly filled adhesives.
Interestingly, the clinical performance of the lightly and
heavily filled adhesives, when used on anterior teeth
and measured by the failure rate of brackets, seems
However, the heavily filled adhesives may be more
effective clinically when bonding the posterior teeth,
where the forces of mastication are heavier.
Because ceramic brackets are usually used on
anterior teeth, it may be advantageous to use lightly
filled adhesives when etching with phosphoric acid.
The clinician should be aware of some important
variables that could influence success when
debonding ceramic brackets.
Force Magnitudes Applied During Debonding, the
mean bond strength for the different bracket,
adhesive, and enamel conditioner combinations
ranged from a low of 40 kg/cm2 to highs in excess of
Most debonding stresses are between 60 and 115
kg/cm2; however, some investigators have reported
forces in excess of 300 kg/cm2.
With metal brackets, the critical question for the
clinician was whether the bond was too weak to
withstand the forces of orthodontic treatment.
With ceramic brackets, clinicians are concerned with
whether the bond was too strong for safe debonding.
Reynolds suggested that a minimum bond
strength of 60 to 80 kg/cm2 was adequate for most
clinical orthodontic needs.
The maximum limit for bond strength has been
Retief reported that enamel fractures can occur with
bond strengths as low as 138 kg/cm 2.
This is comparable with the mean linear tensile
strength of enamel of 148 kg/cm 2.
Therefore, it would seem to be advisable to avoid
tensile bond strengths that are greater than 130
Force Range Related to Debonding When the
"mean" debonding forces in various studies were
evaluated, it became evident that most of the means
fall below the upper limits of what are considered as
safe debonding forces.
However, the potential for clinical disasters lie in the
range of forces that these means actually describe.
The lower values of these ranges (36.0 to 44.0
kg/cm2) pose only one complication, specifically, the
bracket will likely fail during treatment and will need
to be rebonded.
However, the higher values of the range (246.0 to
292.0 kg/cm2) are almost twice as high as the forces
that have the potential for causing significant damage
to the enamel surface.
It is important to note that these wide ranges of forces
occurred regardless of the adhesive tested or the
Unfortunately the clinician when debonding ceramic
brackets cannot predict which of the brackets will have
these extremely high bond strengths.
This poses a clinical dilemma.
In the same patient one could successfully remove all
the brackets except for one tooth. On that one tooth,
enamel cracks or fractures could occur as a result of
the excessive bond strength and the excessive
debonding forces required.
It should be remembered that moisture, temperature,
and other oral variables are known to weaken bond
strength at the enamel-adhesive interface.
Therefore, in vitro bond strength values may be higher
than those obtained in vivo.
This may be an advantage when using ceramic
Combinations of Brackets and Adhesives that will
provide the Clinician With an Optimal Debonding
There are combinations of brackets and adhesives
the clinician should not use.
With a phosphoric acid enamel conditioner and
conventional debonding pliers, the combinations that
produced unacceptably large debonding forces
included chemically or chemically/mechanically
retained ceramic brackets bonded with an unfilled
Similar results were obtained when the
chemically/mechanically retained bracket were bonded
with a highly filled adhesive.
These combinations produced mean debonding force
values exceeding 175 kg/cm2.
Some investigators have found that some chemically
retained ceramic brackets have mean bond strengths
ranging between 198 and 329 kg/ Cm 2 other
combinations produced mean debonding forces less
than 115 kg/cm2, which would appear to be safe
With polyacrylic acid enamel conditioning (crystal
growth), neither the type of adhesive nor the bracket
used was found to be as critical.
This is because bond failure occurs within the crystals
themselves, thus minimizing the stresses transmitted
to the enamel.
Manufacturing companies should be encouraged to
provide the orthodontists with agreed on, standardized
information about their products.
Effectiveness of Various Debonding Methods Because
of the brittle nature of ceramic brackets, earlier
methods of mechanical debonding often cause bracket
or enamel fracture.
As a result, manufacturers, clinicians, and researchers
have attempted to develop new debonding techniques
specifically designed for ceramic brackets;
The earliest types of debonding instruments
used on ceramic brackets applied heavy shear torsion
forces to the already sensitive and mobile teeth.
The sudden nature of bracket failure associated with
such methods had the potential of causing enamel
fracture or cracks.
Swartz stated, "This method of force concentration is
analogous to the delamination of two pieces of bonded
wood. Attempting to twist one piece from the other will
require great forces. Wedging a chisel at the interface
of the two will usually be less destructive and require
significantly less force to separate."
Currently one of the most popular mechanical
debonding techniques used for ceramic brackets
involves applying the blades of a debonding plier near
the enamel surface but within the adhesive.
In the typical in vitro shear bond strength test, the
force is applied on one side of the bracket.
More recently an attempt was made to simulate the
clinical situation and measure the actual force
applied by the pliers during debonding by applying
the force at the bracket-adhesive interface on both
sides of the bracket.
Applying the load to the two sides simultaneously
with the pliers increases the chances of creating a
crack in the brittle adhesive.
The results indicated that this method transmits
one third less force to the enamel compared with a
pure shear force.
This is a very significant reduction in the debonding
force and places much less stress on the enamel
surface, thereby reducing the risk of fracture damage.
The width of the plier blades and debonding forces.
When debonding a ceramic bracket with a sharpedged debonding instrument, the clinician can use
either the 2.0-mm narrow blades or the 3.2-mm wide
The use of narrow blades results in a lower
debonding stress (120 kg/cm2) than with the wider
blades (150 kg/ cm2) ,
In other words, there is a reduction in the debonding
force when using narrow plier blades.
The incidence of enamel cracks after mechanical
In a recent study, transillumination was used to
evaluate damage to enamel surfaces after
The changes evaluated included enamel cracking
Each facial or buccal tooth surface was divided into
nine equal vertical and horizontal zones for detailed
mapping of the enamel cracks.
Most of the teeth, 82%, showed no increase in enamel
cracks after debonding, whereas approximately 18%
of the teeth showed an increase in enamel cracks.
After debonding, the lateral incisors showed the
greatest increase in the number of cracks, 41%. The
molars showed the least increase, 7%.
Teeth bonded with the same adhesive but used in
different forms, for example, either precoated or as a
paste, showed different damage after debonding.
For example, teeth that had precoated brackets
showed the highest increase in the number of cracks
(33%), whereas those bonded with the same adhesive
but used as a paste showed the least (3%).
The difference probably had to do with the consistency
and homogeneity of the precoated adhesives, which
provided for a stronger bond.
It is important to note that the teeth that showed an
increase in the number of cracks had bonds with a
significantly higher mean bond strength (113 kg/cm 2)
than had those teeth that showed no increase in the
number of cracks after debonding (73 kg/ cm 2).
In other words, the stronger the bond strength, the
greater the probability of enamel cracks occurring.
Clinical Precautions When Using Mechanical
Under ideal laboratory conditions, all of the
conventional mechanical debonding techniques were
However, the potential for causing damage is higher if
the integrity of the tooth is already compromised as a
result of preexisting developmental defects, enamel
cracks, large restorations, or with the relatively brittle
Therefore, placement of ceramic brackets should be
avoided in these situations.
The debonding forces result in various degrees of
Clinically these heavy forces are applied at the end of
the active phase of orthodontic treatment to teeth that
are often mobile and sensitive.
To minimize the discomfort and pain, the teeth should
be well protected during bracket removal.
It has been suggested that either the orthodontist
should support the tooth with his or her fingers, or
have the patient bite firmly into a cotton roll to
The likelihood of bracket fracture can be minimized if
the excess composite flash is first removed from
around the bracket.
This will allow the debonding instrument to be fully
seated at the base of the bracket, allowing the plier to
transmit the debonding forces through the strongest
and bulkiest part of the bracket, namely, the bracket
Bracket fracture, when it occurs, is usually quick.
Consequently, fragments could injure the oral mucosa
or the clinician. Furthermore, whole brackets or
fractured bracket particles could become ingested or
aspirated by the patient, creating a significant medical
To minimize such occurrences, it is advisable to
remove the brackets while the mouth is closed and with
a piece of gauze behind the teeth, to catch any loose
In addition, the "flying" projectiles may cause eye injury
to the patient or the clinician. Therefore, protective
eyewear should be used by both the clinician and
Some pliers have a protective sheath that covers the
working end of the instrument. The sheath decreases
the probability of any loose bracket fragments
becoming accidentally discharged into the patient's
Plier blades progressively lose their sharpness,
especially as the blades are abraded from contact
with the much harder ceramic material.
As the plier blades become dull, the debonding
efficiency is significantly reduced.
It is therefore recommended to use new blades after
debonding 50 brackets.
Pliers with non exchangeable blades should be
sharpened on a regular basis.
Alternative Debonding Methods
Alternative methods of debonding ceramic brackets
have been designed to minimize the potential for
bracket fracture or trauma to the enamel surface.
The main purpose of these new methods is to reduce
the force levels during the debonding process.
Three debonding techniques have been proposed:
The ultrasonic technique uses specially designed tips
applied at the bracket-adhesive interface to erode the
adhesive layer between the enamel surface and
bracket base. The resulting force magnitudes needed
with the ultrasonic approach are significantly lower
than those required for the conventional methods of
bracket removal. www.indiandentalacademy.com
However, the ultrasonic technique has a major
Debonding time using this technique is 30 to 60
seconds per bracket, compared with 1 to 5 seconds for
other bracket removal methods.
In addition, there is excessive wear of the relatively
expensive ultrasonic tips.
This wear is the result of the friction between the softer
steel tip moving against the much harder ceramic
surface. There is also the potential for gouging the
enamel surface during the erosion process.
Consequently, this method of ceramic bracket
removal is not yet recommended for clinical use.
Electrothermal debonding instruments are essentially
rechargeable, cordless heating devices that are
placed in contact with the bracket.
The instrument transfers heat through the bracket,
softening the adhesive and allowing bond failure
between the bracket base and the adhesive resin.
This method is a quick and effective way to debond a
Its major disadvantage is related to the relatively high
temperatures generated at the heated tip. Pulpal
damage and mucosal burns are possible.
Debonding ceramic brackets was attempted using both
CO2 and YAG lasers in combination with mechanical
The use of a laser is conceptually similar to the use of
the electrothermal approach, that is, through heat
generation to soften the adhesive.
With the laser, the torque force needed to debond
polycrystalline brackets was lowered by a factor of 27
for molars and a factor of 16 for incisors when
compared with the mechanical debonding forces
used without the laser.
The polycrystalline brackets were illuminated for 2
seconds with a focused CO2 laser beam of 14 W,
whereas the monocrystalline brackets needed only
half that amount of energy.
The laser approach, although still experimental, is
more precise with regard to time and amount of heat
application, and therefore would have better control of
the amount of heat transmitted to the tooth.
A major disadvantage, in addition to the effects of the
thermal energy on the pulp, is the high cost of the
The Effects of Heat Application on the Pulpal Tissues
The short- and long-term effects of electrothermal
debonding on the underlying pulp as well as the
degree of patient discomfort, were evaluated.
Forty-eight premolars planned for orthodontic
extraction were bonded with monocrystalline
brackets and debonded using the electrothermal
Seventeen premolars were not etched or bracketed
and served as controls. Patients were questioned
as to sensations during debonding.
Teeth were extracted at 1 or 4 weeks after bracket
removal and were then histologically examined.
The findings indicated that at the end of 1 week, the
predominant inflammatory cells were lymphocytes,
with no pulpal necrosis observed.
At 4 weeks chronic inflammation decreased over time,
indicating repair of the damaged areas.
The odontoblastic layer was intact, although some
evidence of the earlier damage remained (an
infrequent calciotraumatic line and formation of a
mildly irregular secondary dentin) in 12% of the
A similar reaction occurs when a tooth has a cavity
The histological evidence indicated that the pulp
damage was mostly reversible and the pulp injury,
when it occurred, was relatively mild in the premolar
In the clinical tests, the patients experienced
Generally, the sensation was described as "warmer
than normal body temperature," but was well
An important question that was not answered by the
study was whether the pulp response of premolars
would be similar to that of other groups of teeth.
Premolars have an average enamel/dentin thickness
of 3.6 mm, which essentially acts as insulation
protecting the pulpal tissues.
Incisors have significantly less insulation.
According to data reported by Crispin, at the middle of
the labial surface, the maxillary central incisors have
only 64% as much enamel as the premolars, whereas
the mandibular incisors have only 51% as much
Although the pulp changes were fairly mild in the
premolar specimens, there is a need for further
investigations on the effects of the procedure on the
Rueggeberg and Lockwood also suggested that the
temperature needed to debond brackets varied
significantly, depending on the type of adhesive used.
They suggested thatwww.indiandentalacademy.com
highly filled adhesives will need
more heat to soften and debond.
Ceramic brackets have one main advantage, esthetics.
On the other hand, ceramic brackets have numerous
1. Ceramic brackets have a higher incidence of fracture
during debonding, particularly with the conventional
2. Ceramic brackets are unable to withstand strong
torsional forces, especially after the bracket surface
has been nicked during treatment.
3. The use of ceramic brackets should be avoided on
Therefore, clinicians should conduct a thorough
pretreatment and post treatment examination of the
surface characteristics of enamel using
This is carried out to detect cracks, fractures, or other
defects that may serve as enamel fracture sites
This examination is preventive risk management by
the orthodontist. www.indiandentalacademy.com
4. Enamel wear occurs if ceramic brackets contact
opposing tooth surfaces. Therefore, placement of
ceramic brackets is contraindicated on the lower
anterior teeth in cases with deep overbite and minimal
overjet. In such cases, sufficient overjet has to be
created before bonding the lower incisors. Similarly,
during maxillary incisor retraction, the overbite should
be reduced first so that the maxillary incisors do not
contact the mandibular ceramic brackets.
5. Ceramic brackets can cause nicks in the arch
wires, resulting in more friction between the bracket
and the arch wire. This can decrease the efficiency of
6. The use of ceramic brackets in patients who will
undergo orthognathic surgery should be discouraged.
The fracture of the brackets before, during, or after
surgery creates the potential for undesirable and
7. Because of potential fracture of the bracket or
enamel, the clinician should not delegate the removal
of ceramic brackets to auxiliaries.
There is a demand from patients for ceramic brackets
because of their desirable esthetics, but there is a
need to continue improving current debonding
methods and develop new techniques or design
concepts that are better suited for the removal of
The new techniques need to be reliable and safe, to
both the patient and the orthodontist.
The debonding approach should be tailored to the
type of bracket base retention, bracket design,
enamel conditioner, and/or adhesive used.
The stronger the bond strength between the ceramic
bracket and the enamel, the more critical it is to
consider alternative methods for bracket removal.
Debonding should occur either within the adhesive, or
at the bracket-adhesive interface rather than from the
1. Bishara SE, Trulove TS. Comparisons of different debonding techniques for
ceramic brackets: An in vitro study.
Parts I and II. Am J Orthod Dentofacial Orthop 1990;98: 145-153, 263-273.
la. Strobl K. Bahns TL, Wilham L, et al. Laser-aided debonding of orthodontic
ceramic brackets. Am J Orthod Dentofacial Orthop 1992;152-159.
2. American Association of Orthodontist. Summary of AAO ceramic bracket survey.
The Bulletin Supplement 1989;7: (Winter).
3. Dovgan JS, Walton RE, Bishara SE. Electrothermal debracketing of orthodontic
appliances: Effects on the human pulp. J Dent Res 1990;69:300 (abstr 1531).
4. Swartz ML. Ceramic brackets. J Glin Orthod 1988;22: 82-88.
5. Scott GE. Fracture toughness and surface cracks: The key
to its understanding ceramic brackets. Angle Orthod 1988;58:5-8.
6. Kusy RP. Morphology of polycrystalline alumina brackets and its relationship to
fracture toughness and strength. Angle Orthod 1988;58:197-203.
7. Viazis AD, DeLong R, Bevis RR, et al. Enamel abrasion from ceramic orthodontic
brackets under an artificial oral environment. Am J Orthod Dentofacial Orthop
8. Viazis AD, DeLong R, Bevis RR, et al. Enamel surface abrasion from ceramic
orthodontic brackets: A special case report. Am J Orthod Dentofacial Orthop
9. Pratten DH, Popli K, Germane N, et al. Frictional resistance of ceramic and
stainless steel orthodontic brackets. Am J Orthod Dentofacial Orthop
10. Angolkar PV, Kapila S, Duncanson MG, et al. Evaluation of friction between
ceramic brackets and orthodontic wires of four alloys. Am J Orthod Dentofacial
11. Odegaard J, Segner D. Shear bond strength of metal brackets compared
with a new ceramic bracket. Am J Orthod Dentofacial Orthop 1988;94:201-206.
12. Gwinnett AJ. A comparison of shear bond strengths of metal and ceramic
brackets. Am J Orthod Dentofacial Orthop 1988;93:346-348.
13. Ripley KT. In vitro comparative study of shear and tensile bond strengths for
stainless steel and ceramic orthodontic brackets. Masters Thesis, University of
14. Joseph VP, Rossouw PE. The shear bond strengths of stainless steel and
ceramic brackets used with chemically and light-activated composite resins. Am
J Orthod Dentofacial Orthop 1990,97:121-125.
15. Iwamoto H, Kawamoto T, Kinoshita Z. Bond strength of new ceramic brackets
as studied in vitro. J Dent Res 1987;66:928 (abstr).
16. Hyer KE. An in vitro study of shear and tensile bond strengths comparing
mechanically and chemically bonded ceramic brackets with three bonding agents.
Masters Thesis, University of Iowa, 1989.
17. Swartz ML, Ormco Corporation. A technical bulletin on the issue of bonding and
debonding ceramic brackets. #070-5039, 1988.
18. Viazis AD, Cavanaugh G, Bevis RR. Bond strength of ceramic brackets under
shear stress: An in vitro report. Am J Orthod Dentofacial Orthop 1990;98:214-221.
19. Harris AMP, Joseph VP, Rossouw E. Comparison of shear bond strengths of
orthodontic resins to ceramic and metal brackets. J Glin Orthod 1990;24:725-728.
20. Storm ER. Debonding ceramic brackets. J Glin Orthod 1990;24:91-94.
21. Guess MB, Watanabe LG, Beck FM, et al. The effect of silane coupling agents
on the bond strength of a polycrystalline ceramic bracket. J Glin Orthod
22. Relief DH. The mechanical bond. Int Dent J 1978;28: 18-27.
23. Barkmeier WW, Gwinnett AJ, Shaffer SE. Effects of
reduced acid concentration and etching time on bond
strength and enamel morphology. J Glin Orthod 1987;21:
24. Legier LR, Relief DH, Bradley EL, et al. The effects of
phosphoric acid concentration and etch duration on the
shear bond strength of an orthodontic bonding resin to
enamel: An in vitro study. Am J Orthod Dentofacial
25. Sadowsky PL, Retief DH, Cox PR, et al. Effects of etchant
concentration and duration on the retention of orthodontic
brackets: An in vivo study. Am J Orthod Dentofacial
26. Olsen ME, Bishara SE, Boyer D, et al. Effect of varying
etching time on the bond strength of ceramic brackets. J
Dent Res 1994;73:197 (abstr 766).
27. Smith DC, Cartz L. Crystalline interface formed by
polyacrylic acid and tooth enamel. J Dent Res 1973;52:
28. Maijer R, Smith DC. Crystal growth on the outer enamel
surface: An alternative to acid etching. Am J Orthod
29. Smith DC, Bennett G, Peltoniemi R, et al. Further
of bonding to enamel through crystal growth. J Dent Res
1980; Special Issue B, 995 (abstr 435).
30. Smith DC. LuxJ, Maijer R. Crystal bonding to enamel. J
Dent Res 1981;60:Special Issue A, 178 (abstr 231).
31. Artun J, Bergland S. Clinical trials with crystal growth
conditioning as an alternative to acid-etch enamel
Am J Orthod 1984;85:333-340.
32. Read MJF, Ferguson JW, Watts DC. Direct bonding:
TOC Index << >> Article | Home |
188 Bishara and Fehr
crystal growth as an alternative to acid-etching? Eur J
33. Farquhar KB. Direct bonding comparing a polyacrylic
acid and a phosphoric acid technique. Am J Orthod
34. Burkey PS. Enamel conditioning with acid etch and crystal bonding techniques:
Tensile and shear strength comparisons and scanning electron microscopic
observations. Masters Thesis, University of Iowa, 1985.
35. Bishara SE, FonsecaJM, Fehr DE, et al. Debonding forces applied to ceramic
brackets simulating clinical conditions. Angle Orthod 1994;64:277-282.
36. Reynolds IR. A review of direct orthodontic bonding. Br J Orthod 1979;2:171-178.
37. Maskeroni AJ, Meyers CE, Lorton L. Ceramic bracket bonding: A comparison of
bond strength with polyacrylic acid and phosphoric acid enamel conditioning. AmJ
Orthod Dentofacial Orthop 1990;97:168-175.
38. Gorelick L, Masunaga G, Thomas RG, et al. Round table on bonding. J Glin
Orthod 1978;12:695-714, 761-778, 825-842.
39. Phillips RW. Science of Dental Materials (ed 8). Philadelphia, PA: Saunders,
1982. 40. Phillips HW. JCO/Interviews. J Glin Orthod 1980;14:391- 411.
41. Zachrisson BU, Brobakken BO. Clinical comparison of direct versus indirect
bonding with different bracket types and adhesives. AmJ Orthod 1978;74:62-78.
42. Council on Dental Materials, Instruments, and Equipment: State of the art and
science of bonding in orthodontic treatment. J Am Dent Assoc 1982; 105:844-849.
43. Buzzitta VA, Hallgren SE, Powers JM. Bond strength of
orthodontic direct-bonding cement-bracket systems as
studied in vitro. AmJ Orthod 1982;81:87-92.
44. Faust JB, Grego GN, Fan PL, et al. Penetration coefficient,
tensile strength, and bond strength of thirteen
direct bonding orthodontic cements. Am J Orthod
Dentofacial Orthop 1987;73:512-525.
45. Silverman E, Cohen M, Gwinnett AJ. JCO/Interviews. J
Glin Orthod 1979;13:236-251.
46. Bishara SE, Fehr DE. Comparisons of the effectiveness of
pliers with narrow and wide blades in debonding ceramic
brackets. AmJ Orthod Dentofacial Orthop 1993;
47. Retief DH. Failure at the dental adhesive-etched enamel
interface. J Oral Rehabil 1974;l:265-284.
48. Bowen RL, Rodriguez MS. Tensile strength and modulus
of elasticity of tooth structure and several restorative
materials. J Am Dent Assoc 1962;64:378.
49. Mitchem JC, Turner LR. The retentive strength of
acid-etched retained resins. J Am Dent Assoc 1974;89:
50. Bennett CG, Chiayi S, Waldron JM. The effects of
debonding on the enamel www.indiandentalacademy.com
surface. J Glin Orthod 1984; 18:
Leader in continuing dental education